Presentation on theme: "THE MAINTENANCE STRATEGY AGAINST ROLLING CONTACT FATIGUE University of Belgrade, Faculty of Civil Engineering University of Belgrade, Faculty of Transport."— Presentation transcript:
THE MAINTENANCE STRATEGY AGAINST ROLLING CONTACT FATIGUE University of Belgrade, Faculty of Civil Engineering University of Belgrade, Faculty of Transport and Traffic Engineering Zdenka Popović, PhD, firstname.lastname@example.org Leposava Puzavac, MSc, email@example.com Luka Lazarević, MSc, firstname.lastname@example.org Miloš Ivić, PhD, email@example.com EURO – ZEL 2011 19 th International Symposium 8 th – 9 th, June 2011, Žilina, SK
Dynamic load on modern railways is increasing with speed, traffic and axle load. Defects due to rolling contact fatigue are becoming more expressed because of high wheel/rail contact stress. Freight trains Passenger trains Increase of the axle load Increase of the speed
Rail defects due to rolling contact fatigue in the areas of high wheel/rail contact stress is a marked phenomenon and a problem on the railways worldwide. At first, defects of this type have been observed only on the tracks of heavy haul lines with high axle load. However, nowadays the same occurrence is discerned on conventional lines for mixed traffic as well as on the high speed lines, especially for the speeds over 200 km/h. Wheel/rail contact surface is very small and it measures only 1.5 – 3.0 cm 2. High load is transferred over the small wheel/rail contact surface from the wheel to the rail, which creates high pressure stress.
Rolling contact fatigue is a process of gradual destruction due to the creation and development of an initial crack, until the rail breaks under the influence of variable traffic load. Characteristic look of a steel surface after break caused by rolling contact fatigue
Classification and numbering of rail defects head checking and squat 1st digit2nd digit3rd digit4th digitRail defect type and code 2 (defect away from rail ends) 2 (head) 2 (fissuring) 3 (scaling at the gauge corner) Head checking 2223 7 (cracking and local depression of the running surface) -Squat 227
HEAD CHECKING This defect occurs on the outer rail in the curves of radius up to 3000 m. However, the defect most frequently occurs in the curves of the radius of up to 1500 m. The defect occurs on gauge comer. Defect is distinguished exclusively on tracks with defined motion direction (for example, double track line) and with high quasi-static wheel loads. Fissure orientation depends on the direction of rolling.
Head checking on the double track line shows as fine, short, raked, surface fissures at more or less regular distance, which is usually 1-7 mm (but up to a few centimeters, depending on the rail steel quality). Surface fissures point to existence of fissures already below the surface, extending until certain depth and in certain direction inside the rail head. If the defect is not removed in time, it advances leading to detachment of pieces of rail. Fissure advancing downwards often results in the breaking of rail. Left: Head checking with the scaling (spalling); Right: Rail break caused by the head checking
Fissure propagation due to lubricant penetration
Unless adequate grinding strategy is applied (in the right moment and to the minimum depth necessary), the possibility of fissure advancement to the point of flaking and rail breakage increases many-fold superstructure maintenance costs (early rail replacement, progressive deterioration of the track geometry) and violates reliability and safety of the railway traffic. In practical conditions, periodical cycles of rail grinding according to experience of every railway management solves the problems of not knowing the speed of the fissure development and unreliable fissure depth measurement with the usual ultrasonic inspection procedure. For now, the attention is focused on critical areas (for example outer rail in the curve and similar), which are empirically recognizable by eventual stress concentration, and critical places inside critical areas (for example, gauge corner) where according to experience fissures due to fatigue could be expected.
SQUAT Squats are a rolling contact fatigue phenomenon which occur mainly on straight lines and curves of radius R3000 m with high shear stresses, especially zones where accelerations and breaking occurs. This defect is visible on the running surface of the rail head as a widening and a localised depression of the rail/wheel contact band, accompanied by a dark spot containing cracks with a circular arc or V shape. With time, the crack is expanding towards inner side of the rail head. The cracks propagate inside the head, at first at a shallow angle to the surface. Then, when they reach 3 to 5 mm depth, they propagate downward transversely, producing the fracture of the rail. If the defect is noticed in the initial stadium, grinding can remove it and thus the rail replacement can be deferred. Only in some cases welding can repair this defect. Rail replacement most frequently solves the problem, though.
Example of squat on Serbian railways A typical severe squat (view and cross section)
GRINDING STRATEGIES FOR REMOVAL OF RAIL DEFECTS DUE TO ROLLING CONTACT FATIGUE Grinding strategy applies grinding technique for removing rail steel exposed to fatigue, within limits of tolerances for the corresponding rail profile. The strategy objective is rail life extension, reduction of total track and vehicle maintenance expenses, and railway traffic vibration and noise level control. Preventive, corrective and cyclic activities make the grinding strategy. Preventive activities are undertaken before the defects are noted in the zones where their occurrence is empirically expected. Preventive grinding is applied after laying new rails on the track before acceptance of works. If the rail has to be replaced on the existing track, new rails can be grinded right away or a few weeks after the assembly. It is impossible to completely exclude damage on the upper rail surface by grinding the new rails after they are laid on the track.
Rail head corrugation grinding and grinding of phenomena due to rolling contact fatigue are corrective activities. These activities are planned and applied when the established tolerance limit for the corresponding defect is exceeded. Cyclical activities remove a thin layer (0.1 to 0.2 mm) from the entire head surface, i.e. up to 0.6 mm in the damage zones. Rail cross profile corrections are performed within the narrow tolerance limits, ± 0.3 mm. In the past few years special modified rail cross profile, so called "anti head checking profile", has been applied in Europe. So far there is no unique anti head checking rail profile, but for their own needs and according to their own experience, every railway management develops a rail profile by re-profiling standard rail profiles manufactured according to EN 13674-1: 2003: Railway applications - Track - Rail - Vignole railway rails 46 kg/m and above.
CONCLUSIONS Defects illustrated in this paper are not included in the Serbian technical regulations. This paper emphasizes that the optimum test interval is based on the local conditions: superstructure construction, vehicle speed, axle load and traffic load. Foreign strategies cannot be uncritically accepted. Preventive, corrective and cyclic grinding is recommended as a measure to prolong rail life, decrease total track and vehicle maintenance expenses, control railway traffic vibration and noise levels, according to European standards. An urgent harmonization of railway maintenance regulations with European regulations is necessary for pursuing the conclusions of this paper, while respecting local specifics and limitations.
This work was supported by the Ministry of Science and Technological Development of Republic of Serbia through the research project No. 36012: Research of technical-technological, staff and organisational capacity of Serbian Railways, from the viewpoint of current and future European Union requirements. Ďakujem vám za pozornosť! Thank you for your attention!